From https://focenter.com/cross-sectioning-service/ Fiber Optic Connector Cross Sectioning and Analysis observations from “Connector B” notes
Observations: This connector has (1) distinctive fiber fracture at the beginning of the ceramic internal chamfer (photo B.2). I did notice more than usual “epoxy shrinkage” against the walls internally. This shrinkage during the thermal curing contributed to the fiber fracture where a nick fatigued the fiber and the stresses of thermal curing and shrinkage actually separated the fiber at this location. The remaining fiber trapped inside the shaft of the ferrule acted as an anchor point. This is the most common problem created by the nicking of the fiber from the improper use of mechanical strippers or misaligned blades.
Additional resources from the FOC team include:
- Category Resource:
- Glossary, Acronyms, Military Specifications for Connectors: http://bit.ly/2a2EFn8
- Q&A Resource: email technical questions to AskFOC@focenter.com
Have questions about this FOC Tip?
Contact FOC with questions at: (800) 473-4237 / 508-992-6464 or email: FiberOpticCenter@focenter.com and we will respond ASAP.
- Lapping film options, part 2 - May 18, 2020
- Standards for optical cable assembly manufacturers - May 7, 2020
- Key specifications of connectors - January 3, 2020
- Considerations regarding freezing epoxy – implementing process adjustment - December 16, 2019
- Considerations regarding freezing epoxy – THAWING - November 13, 2019
- Crystallization in Epoxies: How to Identify and Reverse it - October 23, 2019
- Measuring Insertion Loss and Return Loss Recommendations to Achieve the Best and Most Accurate Test Measurement - October 23, 2019
- Cross-Sectioning Fiber Optic Connectors: An Effective Diagnostic Method to Identify Defects and Resolve Process Issues - October 23, 2019
- The “Ideal” Fiber Height for a Fiber Optic Connector – and How to Achieve It - October 23, 2019
- Considerations regarding freezing epoxy – recommended length of time - October 23, 2019